A Flexible Fluorescent SCC-MOF for Switchable Molecule Identification and Temperature Display
Dong, Xi-Yan; Huang, Hui-Lin; Wang, Jia-Yin; Li, Hai-Yang; Zang, Shuang-Quan; Chemistry of Materials 30 (2018) 2160–; doi:10.1021/acs.chemmater.8b00611

data_4002894
_publ_section_title
;
 A Flexible Fluorescent SCC-MOF for Switchable Molecule Identification and
 Temperature Display
;
_journal_issue                   6
_journal_name_full               'Chemistry of Materials'
_journal_page_first              2160
_journal_paper_doi               10.1021/acs.chemmater.8b00611
_journal_volume                  30
_journal_year                    2018
_chemical_formula_moiety         'C60 H82 Ag10 F6 N4 O10 P2 S6'
_chemical_formula_sum            'C60 H82 Ag10 F6 N4 O10 P2 S6'
_chemical_formula_weight         2466.29
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_audit_creation_date             2017-07-27
_audit_creation_method
;
Olex2 1.2
(compiled 2016.11.07 svn.r3352 for OlexSys, GUI svn.r5261)
;
_cell_angle_alpha                62.160(2)
_cell_angle_beta                 88.3470(10)
_cell_angle_gamma                79.9020(10)
_cell_formula_units_Z            1
_cell_length_a                   11.9522(2)
_cell_length_b                   14.1064(2)
_cell_length_c                   14.2144(2)
_cell_measurement_reflns_used    13022
_cell_measurement_temperature    130.01(10)
_cell_measurement_theta_max      72.4060
_cell_measurement_theta_min      3.6710
_cell_volume                     2082.49(7)
_computing_cell_refinement       'CrysAlisPro 1.171.39.7b (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.39.7b (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.39.7b (Rigaku OD, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      130.01(10)
_diffrn_detector                 'CCD plate'
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  t~exp~   \w     \q     \k     \f   Frames
--------------------------------------------------------------------------
  1  \w      7.00  74.00   0.25    0.25    --   45.20  77.00-120.00  268
  2  \w    -10.00  66.00   0.25    0.25    --   45.20 -57.00  30.00  304
  3  \w     98.00 125.00   0.25    0.25    --   45.20  57.00 120.00  108
  4  \w     91.00 130.00   0.25    0.25    --   45.20  77.00-120.00  156
  5  \w     15.00 125.00   0.25    0.25    --   45.20  57.00-150.00  440
  6  \w     35.00  96.00   0.25    0.25    --   45.20  57.00 120.00  244
  7  \w     30.00  93.00   0.25    0.25    --   45.20  57.00 -30.00  252
  8  \w     11.00  55.00   0.25    0.30    --  100.80 -61.00-150.00  176
  9  \w     66.00 133.00   0.25    0.30    --  100.80 -82.00  60.00  268
 10  \w     21.00 123.00   0.25    0.30    --  100.80 -82.00-150.00  408
 11  \w     95.00 190.00   0.25    0.30    --  100.80  30.00 -90.00  380
 12  \w     91.00 168.00   0.25    0.30    --  100.80  77.00 150.00  308
 13  \w     12.00  49.00   0.25    0.30    --  100.80 -82.00 120.00  148
 14  \w     80.00 119.00   0.25    0.30    --  100.80 -82.00 120.00  156
 15  \w     11.00  51.00   0.25    0.30    --  100.80 -82.00  60.00  160
 16  \w     14.00 108.00   0.25    0.30    --  100.80 -61.00  60.00  376
 17  \w     99.00 169.00   0.25    0.30    --  100.80  45.00-180.00  280
 18  \w     62.00 120.00   0.25    0.30    --  100.80 -61.00-150.00  232
 19  \w     15.00  98.00   0.25    0.30    --  100.80 -61.00 -30.00  332
 20  \w     24.00 114.00   0.25    0.30    --  100.80 -82.00 -30.00  360
 21  \w     56.00 188.00   0.25    0.30    --  100.80  30.00 -60.00  528
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'XtaLAB Pro: Kappa single'
_diffrn_measurement_method       '\w scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0331712000
_diffrn_orient_matrix_UB_12      0.1247095000
_diffrn_orient_matrix_UB_13      -0.0674717000
_diffrn_orient_matrix_UB_21      -0.1095723000
_diffrn_orient_matrix_UB_22      -0.0013888000
_diffrn_orient_matrix_UB_23      0.0600656000
_diffrn_orient_matrix_UB_31      0.0640155000
_diffrn_orient_matrix_UB_32      0.0151075000
_diffrn_orient_matrix_UB_33      0.0831749000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0328
_diffrn_reflns_av_unetI/netI     0.0391
_diffrn_reflns_Laue_measured_fraction_full 0.992
_diffrn_reflns_Laue_measured_fraction_max 0.992
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            17601
_diffrn_reflns_point_group_measured_fraction_full 0.992
_diffrn_reflns_point_group_measured_fraction_max 0.992
_diffrn_reflns_theta_full        64.997
_diffrn_reflns_theta_max         64.997
_diffrn_reflns_theta_min         3.523
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Cu) X-ray Source'
_exptl_absorpt_coefficient_mu    20.732
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.25509
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.39.7b (Rigaku Oxford Diffraction, 2015)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colourless
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    1.967
_exptl_crystal_description       block
_exptl_crystal_F_000             1200
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.19
_exptl_crystal_size_min          0.08
_refine_diff_density_max         2.010
_refine_diff_density_min         -1.178
_refine_diff_density_rms         0.130
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.037
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     479
_refine_ls_number_reflns         7028
_refine_ls_number_restraints     51
_refine_ls_restrained_S_all      1.049
_refine_ls_R_factor_all          0.0409
_refine_ls_R_factor_gt           0.0384
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0607P)^2^+4.2424P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1018
_refine_ls_wR_factor_ref         0.1036
_reflns_Friedel_coverage         0.000
_reflns_number_gt                6522
_reflns_number_total             7028
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            cm8b00611_si_003.cif
_cod_data_source_block           ag10bpy_dry_130k
_cod_depositor_comments
'Adding full bibliography for 4002893--4002902.cif.'
_cod_original_cell_volume        2082.49(6)
_cod_database_code               4002894
_chemical_oxdiff_formula         'C H O N S Ag'
_reflns_odcompleteness_completeness 98.99
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     66.97
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
 At 1.5 times of:
  All C(H,H,H) groups, All O(H) groups
2. Restrained distances
 F1-C30 \\sim F3B-C30 \\sim F3-C30 \\sim F2B-C30 \\sim F2-C30 \\sim F1B-C30
 with sigma of 0.01
3. Uiso/Uaniso restraints and constraints
Uanis(F1B) \\sim Ueq, Uanis(F1) \\sim Ueq, Uanis(F3B) \\sim Ueq, Uanis(F3)
\\sim Ueq, Uanis(F2B) \\sim Ueq, Uanis(F2) \\sim Ueq: with sigma of 0.01 and
sigma for terminal atoms of 0.02
4. Others
 Fixed Sof: F1(0.5) F1B(0.5) F2(0.5) F2B(0.5) F3(0.5) F3B(0.5)
5.a Aromatic/amide H refined with riding coordinates:
 C13(H13), C14(H14), C16(H16), C17(H17), C18(H18), C19(H19), C21(H21),
 C22(H22), C24(H24), C25(H25), C26(H26), C27(H27), C28(H28)
5.b Idealised Me refined as rotating group:
 C2(H2A,H2B,H2C), C3(H3A,H3B,H3C), C4(H4A,H4B,H4C), C6(H6A,H6B,H6C), C7(H7A,
 H7B,H7C), C8(H8A,H8B,H8C), C10(H10A,H10B,H10C), C11(H11A,H11B,H11C), C12(H12A,
 H12B,H12C)
5.c Idealised tetrahedral OH refined as rotating group:
 O5(H5)
comments: The relatively large space in this structures brought the 
disorder of the terminal group trifluoroacetate anion. 
The atoms F1, F2, and F3 of the trifluoroacetic acid anions were 
located at two orientations with a fixed occupancy ratio of 0.5:0.5. 
Their ADP and relevant C&#x00A8;CF bond lengths were restrained 
by "ISOR 0.01" , "SIMU 0.01" and "SADI 0.01", respectively.
;
_shelx_shelxl_version_number     2016/6
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
- Detector area scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 3.280
_oxdiff_exptl_absorpt_empirical_full_min 0.630